Download Presentation

Update on charge collection measurements with SCT128 chip in Ljubljana

112 Views

Download Presentation
## Update on charge collection measurements with SCT128 chip in Ljubljana

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -

**Update on charge collection measurements with SCT128 chip in**Ljubljana • Igor Mandić1, Vladimir Cindro1, Andrej Gorišek1, Gregor Kramberger1, Marko Milovanović1, Marko Mikuž1,2, Marko Zavrtanik1 • 1Jožef Stefan Institute, Ljubljana, Slovenia • 2 Faculty of Mathematics and Physics,University of Ljubljana, Slovenia 7th “Trento” Workshop on Advanced Silicon Radiation Detectors (3D and P-type Technologies) Jožef Stefan Institute, Ljubljana, Slovenia, 29.2. – 2.3. 2012.**Introduction:**• charge collection measurements with 90Sr source on SCT128 chipsetup in Ljubljana • accelerate annealing: repeat charge collection measurements (at -20°C) after several annealnig • steps at 60° C • ATLAS07 mini strip detectors produced by Hamamatsu irradiated with pions at PSI in 2010 • and with neutrons in Ljubljana • p-type, 6 inch FZ wafer, 320 µm thick, 75 µm strip pitch, 1x1 cm2, Vfd ~ 190 V • many results of measurements with these detectors already published: • annealing studies with neutron irradiated detectors published in: • I. Mandić et al., NIM A 629 (2011) 101–105 • annealing studies with pion irradiated detectors published in: • I. Mandić et al., 2011 - JINST - 6 - P11008 • Outline of this presentation: • - short summary of annealing measurements with pionandneutron irradiated detectors • - measurements with mixed irradiated detector: pions at PSI + neutrons in Ljubljana • - time dependence of collected charge I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Shown in the last RD50 workshop(19thRD50 Workshop, CERN, 21**– 23November 2011) : http://indico.cern.ch/getFile.py/access?contribId=4&sessionId=2&resId=1&materialId=slides&confId=148833 Neutrons: t ~ 500 minutes, V ~ 1300 V Pions: t ~ 5000 minutes, V ~ 1300 V • multiplication obvious in detectors irradiated with pions after longer annealing times • then after irradiation with neutrons: • smaller stable damage and reverse annealing introduction rates for pions takes longer to • reach sufficient Neff for high enough peak electric field for multiplication I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Vfd (estimated from the kink in the Q-V plot) after 80**minutes at 60°C • gc = 0.017 cm-1 measured for FZ-p type material irradiated with neutrons • (G. Kramberger et al,. NIMA 612 (2010) 288-295, V. Cindro et al., NIMA 599 (2009) 60-65) • pions compatible with gc ~ 0.005 cm-1 • significantly smaller than for neutrons • lower Vfd increase after proton irradiation of HPK sensors measured also by • K. Hara et al.,Nucl. Instr. Meth. A 636 (2011) S83-S89. I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**compare with Hamburg model,long term annealing described**by: pions • with τY = 1100 min (G. Kramberger et al.) better agreement with gY= 0.02 cm-1 than with gY ~ 0.05 cm-1 • measured for p-type FZ material irradiated with pions (byG.Kramberger et al.) • other parameters used in theHamburg model: gc ~ 0.005 cm-1 , Vfd,0 = 170 V, ga = 0.018 cm-1 , τa = 19 min I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**pad detector geometry, uniformNeff, V < Vfd :**ifV > Vfd • annealing of Neffaccording to Hamburg model neutrons pions multiplication “threshold” • multiplication after: - few hundred minutes on 60°C for neutrons (Φeq = 1e15 n/cm2 ) • - few thousand minutes on 60°C for pions (Φeq = 1.6e15 n/cm2 ) • agrees with measurements I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Mixed irradiation**• mixed: 1.Φeq = 4.6e14 n/cm2 , pions, annealed for 41 h at 60°C Neff ~ 1.1e13 cm-3 • 2.Φeq= 5.4e14 n/cm2 , neutrons, annealed 80 min. at 60°C Neff ~ 2.3e13 cm-3 • Sum: Neff ~ 3.4e13 cm-3 • neutrons: Φeq= 1e15 n/cm2 , annealed for 80 min. at 60°C Neff ~ 3.3e13 cm-3 • trapping: mixed: τe = 2.3 ns, τh = 1.6 ns • neutrons: τe = 2.3 ns, τh = 2.2 ns • result consistent: similar Neff and similar τe,h similar collected charge**Mixed irradiation**• accelerated annealing at 60 C with mixed irradiated detector multiplication effects visible after 1200 minutes of annealing I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Mixed irradiation**• multiplication affects also detector current and noise I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Exercise:plot collected charge vs. Neff**• lines connect measurements after different annealing steps • Neff calculated using Hamburg model with following parameters: • pions: Vfd,0 = 170 V, ga = 0.018 cm-1 , τa = 19 min,gc ~ 0.005 cm-1 , gY ~ 0.02 cm-1 , τY = 1100 min • neutrons: Vfd,0 = 170 V, ga = 0.018 cm-1 , τa = 19 min,gc ~ 0.017cm-1,gY ~ 0.05 cm-1 ,τY = 1100 min • increase of Neff by reverse annealing may lead to increase or decrease of MPV, depending on bias • voltage and fluence • “sharp” increase of MPV with annealing (due to multiplication) seen if Neff > 3e13 cm-3 and V > 1300 V • increase of Neff with irradiation decreases MPV trapping I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Exercise: plot collected charge vs. Emax**• MPV vs. maximum electric field (in pad detector geometry, uniform Neff): • If Emax > 12 V/µm MPV doesnotdecrease with annealing • Emax ~ 12 V/µm threshold for multiplication Neffor Emax are not sufficient parameters to describe the behavior electric field in heavily irradiated detector more complicated (polarizationeffects …) see the 3D TCT results see V. Eremin et al., NIMA 658 (2011) 145-151, M. Mikuž et al., NIMA 636 (2011) S50-S55 I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Time dependence**• changes of ChargeCollection with bias history and time reported at the last RD50 workshop Adrian Driewer: Alibava Multiplication fades with time NicolaPacifico: Edge TCT Multiplication not seen after biasing the detector with high current (700 uA). Comes back after heating the detector to RT I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Time dependence**• detector irradiated to Φeq= 1.6 ∙1015neq/cm2 with pions, annealed for 84 hours at 60°C • bias 1300 V (multiplicationobserved at this bias) • measure collected charge with SCT128 at T ~ -20°C • charge collection measurements repeated every few hours, bias 1300 V continuously on Two measurements: before and after applying forward bias (I = 750 µA) Heat to RT Bias off, T ~ -20 C**spectrum of cluster signals changes with time on bias:**I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**detector current changes with time on bias**• detector current measured from voltage drop on a resistor in high voltage • power supply line • guard ring not bonded Bias off Heat to RT After applying forward bias (I = 750 µA) I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**bias dependence of Neff measured before:M. Mikuž et al.,**NIMA 466 (2001) 345 • FZ n-type diodes irradiated to 2e11 n/cm2 • time constant for Neff rise • after bias switched on at T = 20°C • τ ~ 60 h • time constant at T = -7 C • τ ~ 2700 h I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**G. Kramberger etal., NIMA 600 (2009) 555**• n-type MCz and epitaxial diodes • annealed 500 h (MCz) and 20000 h (Epi) at RT • T = -8°C , fit with two exponentials, with short and long time constants • τs ~ 8 h, τL ~ 700 h • τs ~ 10 h, τL~ 260 h • at T = -8°Cτs ~ 10 h and τs ~ 8 h • at T = 20° C τs ~ 0.8 h and τs ~ 3.6 h • we measure τ ~ 30 h at T ~ -20°C so maybe it is a related effect • but: increase of Neff should increase collected charge if multiplication is on I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Summary**• in ATLAS07 Hamamatsu p-type mini strip detectors irradiation with pions causes • smaller increase of Vfdthan irradiation with neutrons • increase of Vfdwith long term annealing slower than after irradiation with neutrons • both can be expected for oxygenated FZ material • CCE and annealing behavior of mixed irradiated detector as expected from • measurements with neutron and pion irradiations • CCE and detector current change with time on bias: • collected charge falls with time on bias with time constant τ ~ 30 h at T = -20° C, • could be the consequence of the “bistability” effect • changes of detector current with time observed I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**exercise: plot detector current vs. Emax**• threshold at aboutEmax ~ 12 V/µm • threshold ?? I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012**Detectors:**• p-type, 6 inch FZ wafer, 320 µm thick, 75 µm strip pitch, 1x1 cm2, Vfd ~ 170 V • produced by Hamamatsu • ATLAS07-PSSSD_Series I, batch number: VXX73414 • 1. mixed irradiation: A07, W49, Z1, P19 • - pions at PSI: Φ = 4.14∙1014π /cm2= 4.6 ∙1014neq/cm2 • - neutrons in Ljubljana:Φ= 5.4 ∙1014neq/cm2 • 2. time dependence: A07, W22, Z3,P1 • - pions at PSI Φ = 1.43∙1015π /cm2= 1.6 ∙1015neq/cm2 I. Mandić, 7th "Trento" Workshop on Advanced Radiation Detectors, Ljubljana, 2012